# Viscoelastic properties

## Presentation on theme: "Viscoelastic properties"— Presentation transcript:

Viscoelastic properties
Polymers have both ideal elastic and viscous behavior depending on time and temperature.

Ideal (elastic) Solid Hooks Law
response is independent of time and the deformation is dependent on the spring constant.

Ideal Solid

Ideal Liquid h= viscosity de/dt = strain rate
The viscous response is generally time- and rate-dependent.

Ideal Liquid

The behaviour of linear elastic were given by Hooke’s law:
or The behaviour of linear viscous were given by Newton’s Law: E= Elastic modulus s = Stress e= strain de/dt = strain rate ds/dt = stress rate h= viscosity ** This equation only applicable at low strain

Viscoelastic behavior
Behaviour of most polymer is in between behaviour of elastic and viscous materials. At low temperature & high strain rate, Polymer demonstrate elastic behaviour, At high temperature & low strain rate, Polymer demonstrate viscous behaviour At intermediate temperatures & rate of strain Polymer demonstrate visco-elastic behaviour

Polymer is called visco- elastic because:
Showing both behaviour elastic & viscous behaviour Instantaneously elastic strain followed by viscous time dependent strain Load released elastic Load added viscous viscous elastic

Maxwell Model

Kelvin Voigt Model

Burger Model

Static Modulus of Amorphous PS
Glassy Leathery Rubbery Viscous Polystyrene Stress applied at x and removed at y

Dynamic Mechanical Analysis

Spring Model g = g0⋅sin (ω⋅t) g0 = maximum strain w = angular velocity
Since stress, t, is t = Gg t = Gg0sin(wt) And t and g are in phase

Whenever the strain in a dashpot is at its maximum, the rate of change of the strain is zero ( g = 0). Whenever the strain changes from positive values to negative ones and then passes through zero, the rate of strain change is highest and this leads to the maximum resulting stress. Dashpot Model

Kelvin-Voigt Model

Dynamic (Oscillatory) Testing
In the general case when the sample is deformed sinusoidally, as a response the stress will also oscillate sinusoidally at the same frequency, but in general will be shifted by a phase angle d with respect to the strain wave. The phase angle will depend on the nature of the material (viscous, elastic or viscoelastic) Input Response where 0°<d<90° stress strain viscosity Gmodulus 3.29

Dynamic (Oscillatory) Testing
By using trigonometry: (3-1) In-phase component of the stress, representing solid-like behavior Out-of-phase component of the stress, representing liquid-like behavior Let’s define: where: 3.30

Physical Meaning of G’, G”
Equation (3-1) becomes: We can also define the loss tangent: For solid-like response: For liquid-like response: G’storage modulus G’’loss modulus

Real Visco-Elastic Samples

Typical Oscillatory Data
G’ G’’ log G log  Rubber G’storage modulus G’’loss modulus Rubbers – Viscoelastic solid response: G’ > G” over the whole range of frequencies

Typical Oscillatory Data
G’ G’’ log G log  Melt or solution G0 Less liquid like G’storage modulus G’’loss modulus More liquid like Polymeric liquids (solutions or melts) Viscoelastic liquid response: G” > G’ at low frequencies Response becomes solid-like at high frequencies G’ shows a plateau modulus and decreases with w-2 in the limit of low frequency (terminal region) G” decreases with w-1 in the limit of low frequency

Blend

Epoxy

Nylon-6 as a function of humidity

E’storage modulus Polylactic acid E’’loss modulus

Tg 87 °C

Tg -123 °C (-190 F) Tm 135 °C (275 F)

Polyurethane foam (Tg 160 C)
G’storage modulus Polyurethane foam (Tg 160 C) G’’loss modulus

G’storage modulus G’’loss modulus These data show the difference between the behaviour of un-aged and aged samples of rubber, and were collected in shear mode on the DMTA at 1 Hz. The aged sample has a lower modulus than the un-aged, and is weaker. The loss peak is also much smaller for the aged sample.

Tan d of paint as it dries

Epoxy and epoxy with clay filler

Dynamic test of a Voigt solid

Benefits of Dynamic Testing